Alkali-activation of tungsten mining waste mud
blended with waste glass: reactivity, performance
and innovative applications
The World is facing serious environment problems caused by global warming and climate changes, mainly because of the increase of carbon dioxide (CO2) in the atmosphere .
Approximately 5–7% of global anthropogenic CO2 emissions results of the manufacturing of
Ordinary Portland cement (OPC) [2,3]. In 2016, the global anthropogenic CO2 emissions
increased approximately 8% with an estimated total value of about 1.45 ± 0.20 Gt CO2 .
Consequently, the development of alternative low‑carbon binders is recognized as a smart option to reduce CO2 emissions . The alkali-activated materials (AAM) technology brings a
new type of cementing materials that don’t produce CO2 emissions like the case of Portland
cement (PC) industry . Thus, there is a growing demand to replace PC concrete by alkali-activated concrete. In fact, these innovative alkali-alkali-activated construction materials under certain conditions have lower greenhouse gas emissions, causing lower environmental impacts and CO2 emissions that are associated with their manufacture .
Household and industrial waste management remains an issue worldwide particularly in Europe. European economic activity and households produced 2.5 billion tons of wastes in 2012, which 62% comes from construction and mining and quarrying activities, while manufacturing, households, energy and other economic activities produce the other 38%. Mines and quarries waste accounts for about 28% of the total generated waste from industrial processes and households in the EU . Most mining and quarrying and other industrial wastes can be reused in earthworks and construction, namely the coarser fractions into asphalt pavements and concrete . It can also become raw material for industrial applications where the high value of the product does not prejudice its reuse due to transport costs . Other research studies have been focused in developing technical-artistic value added and polymer-based composite materials .
The reuse of fine particles from mud tailings as precursor materials for alkali-activated binders and applications have also been conducted and are very promising from a technical, environmental and economic point of view [12,13]. Besides, the alkaline activation of aluminosiliceous industrial by-products is widely known to yield binders whose properties make them comparable to or even stronger and more durable than ordinary Portland cement [14–16]. Besides, several non-conventional waste materials are re-used nowadays as precursors in the alkaline activation, that can be blended/combined with mining waste mud tailings with promising results .
This study evaluated the results to produce alkali-activated binders (AAB) by blending tungsten mine waste mud (TMW) and fine waste glass (WG) activated with a composition of sodium silicate (SS) and sodium hydroxide (SH). This research work is part of REMINE research program (H2020 RISE-Marie Curie Action) that aims to the reuse of mining waste into innovative geopolymeric-based structural panels, precast, ready mixes and in-situ applications. The project is coordinated by Beira Interior University (PT) with the following partners: Brunel University (UK), Silesian University (PL) Bologna University (IT), Granada University (SP), Strathclyde University (UK), Kiev National University of Civil Engineering and Architecture (UA), Alsitek Ltd (UK). Sofalca, Lda (PT), Beira Serra (PT)) .
Some potential uses of these new materials obtained from alkali-activation of tungsten mud waste and other precursor materials, as well incorporating expanded granulated cork, such us
a safety barrier, a high energy efficient panel for a vegetated surface, and a foamed lightweight brick wall are presented [19,20].
The main materials used in this investigation consisted of tungsten mine waste mud (TMW) from Panasqueira mine in Covilhã, Portugal, milled waste glass (WG), sodium hydroxide (NaOH) (SH), and sodium silicate (Na2 SiO3) (SS). Some specimens tested in this research also included
tungsten mine coarse wastes (TCW), metakaolin (MK), granulated expanded cork (GC) and aluminum powder (AL). Metakaolin was provided by the German chemical company BASF, while GC was supplied by Sofalca Lda, located in Abrantes, Portugal). The study was carried on using natural (as obtained in deposit) (N-TMW) and heat-treated (950ºC for two hours) (C-TMW) tungsten mine waste mud. WG was produced after milling for 6 hours using a ball mill. Both TMW and WG were used with particle size lower than 300µm, obtained by sieving analysis. The chemical composition of the TMW and WG was obtained by SEM-EDS. Table 1 shows the average values of TMW (natural and thermal treated) and WG chemical composition. The density of precursor materials was obtained by helium pycnometer (Micromeritics AccuPyc 1330). TMW density was 3,031 g/cm3 for N-TMW and 2,950 g/cm3 for C-TMW. Specific surface was obtained
by the Blaine method (ACMEL LABO BSA1). C-TMW specific surface is slightly lower (2117 cm2/g)
than N-TMW (2417 cm2/g). Grain size distribution analysis was made for TMW and WG by laser
diffraction analysis. The TMW has a mean particle size of 12,1 µm (N-TMW) and 16,3 µm (C-TMW) while the WG has a mean particle size of 39,7 µm. Sodium hydroxide solution was prepared by dissolving sodium hydroxide pellets (98% purity obtained from Fisher Scientific, Schwerte, Germany) in deionized water and allowed to cool before use. Sodium silicate (obtained from Solvay SA, Póvoa de Santa Iria, Portugal) had a SiO2/Na2O = 3.23 (8.60% by
weight Na2O, 27.79% by weight SiO2, 63.19% by weight H2O, and 0.4% by weight Al2O3). Table 1- Chemical composition (% by weight) of TMW and WG determined by SEM-EDS
(Supra 35VP/EDAX, Oberkochen, Germany)
Chemical compound N-TMW C-TMW WG MK SiO2 49.33 49.66 73.93 52.28 Al2O3 16.28 14.42 0.00 42.99 Fe2O3 13.67 22.44 0.40 1.49 SO3 8.93 4.70 0.00 0.00 K2O 4.38 4.44 0.69 0.94 Na2O 0.64 0.44 9.72 0.32 CaO 0.83 0.97 12.83 0.00 MgO 4.93 1.80 0.00 0.47 TiO2 1.00 1.13 0.00 0.00
2.2. Mixing and curing conditions
All sample preparation was carried on at room temperature (around 20ºC). Alkali activated binders (AAB) were produced by blending TMW with WG and MK, with different percentages. For the constituents of the AAB the following parameters were selected: Molarity of SH= 10M; Weight ratio of SS:SH=4 and Weight ratio of precursor/activator = between 2.8 to 3 (except for samples containing higher percentage of MK were lower ratio, between 1 to 2, was used). To produce AAB samples TMW, WG and MK were first mixed in dry state for about 3 minutes. The SS and SH were also mixed together for a period about 5 minutes. Then alkali-activator solution was stirred together with the dry mix for about 5 minutes. To produce Alkali activated concrete (AAC) tungsten coarse wastes (TCW) were added to the composition and mixed in the dry state with TMW and WG, before adding the activator solution. To produce lightweight
alkali-activated materials (L-AAM) granulated expanded cork (GC) was added to the mixture of TMW and WG and stirred in the dry state. To produce foamed alkali-activated materials (F-AAM) aluminum powder (AL) was added with different percentage to the dry mix (TMW, WG, MK) and mixed with all together for additional one minute. The resulting AAB, AAC, L-AAM F-AAM mixes were then placed in prismatic molds of different sizes (accordingly to different tests) and cured in oven at 60ºC for 24 hours, prior to testing. Most details of mix preparation and curing procedures were developed in previous studies .
3. Results and discussion
3.1. Binders compressive strength
The mechanical properties of alkali-activated binders (AAB) were evaluated by compressive strength testing. The formation of organic compounds was analyzed by Fourier Transforms Infrared Spectroscopy (FTIR). The highest compressive strength (65 MPa at 28 days) was achieved for samples containing 20% waste glass, as presented in figure 1. Overall, the best mechanical behavior was found out on binder specimens with natural waste mud (N-TMW) instead of C-TWM. AAB produced with less than 25% waste glass exhibit a very good mechanical behavior, at 28 days, increasing strength along time. On the other hand, AAB mixes containing more than 25% WG (higher CaO content) showed a decrease in compressive strength over time. While, AAB containing less than 5% waste glass showed a slow alkaline activation reaction. The FTIR analysis revealed a reduction in the absorption intensity, of the main bands, for lower TMW content and along curing time. It indicates that higher WG content and time of curing led to the further dissolution of Si-O from the TMW.
Figure 1 – Compressive strength at 28 days of AAM containing between 5 to 40% WG
3.2. Reactivity based on chemical leaching
Reactivity of AAB’s with different composition was evaluated by chemical leaching based on electrical conductivity measurements. For this procedure 2.5 x 2.5 x 2.5 cm cubic specimens were used, after being cured for 7 days. First, specimens to be tested were placed in a goblet containing distilled water at a constant level of 150 ml. Then the electrical conductivity was measured by means of a probe that recorded values from hour to hour until reaching a constant electrical conductivity value. Since the electrical conductivity changes with the number of free ions that migrated from the samples to the distilled water, the higher the sample conductivity, the lower the alkaline activation reactivity extent.
Thus,from table 2 results we can conclude
that the best reaction can be obtained on AAB mixes where TMW is replaced by 10% weight of both WG and MK (i.e. AAB mix = 80%N-TMW + 10%WG + 10%MK).
Table 2. Electrical conductivity of AAB mixes, containing N-TMW, WG and MK
AAB mix composition Conductivity (µs/cm)
Number of hours to reach a constant
conductivity value 20%N-TMW + 80%WG 14014 99 50%N-TMW + 50%WG 17781 330 80%N-TMW + 20%WG 15894 50 80%N-TMW + 10%WG + 10%MK 12908 64 100% N-TMW 14610 428 100% WG 10000 66 100% MK 4122 40
3.3. Thermal resistance after 800ºC temperature exposure
Thermal resistance of AAB’s was evaluated after being exposed to 800ºC temperature, for 2 hours’ period. For this study, 15 different AAB mixes were produced (see table 3) with a precursor/activator ratio of 2.85, except for mixtures 100%MK and 50%WG+50%MK where this ratio was 1.1 and 2.17, respectively. Compressive strength tests were performed on cubic specimens with 4 cm size and were carried on in two phases. Initially, AAB specimens were tested for compressive strength. Later, specimens with the same chemical composition were tested for compressive strength after being exposed to 800°C temperature, for 2 hours’ period. A static furnace (muffle) was used for the temperature exposure. Before the exposure period (800ºC for 2 hours), the temperature was gradually increased. Based on results obtained, most of AAB’s produced with N-TMW, WG and MK present an increase of compressive strength when exposed to 800ºC. Besides the presence of GC, as a lightweight aggregate, is also beneficial regarding the increase of compressive strength of different AAB’ mixes after being exposed to 800ºC.
Table 3. Thermal resistance of AAB mixes at 800ºC, containing N-TMW, WG, MK and GC
ABB mix composition Weight loss (%)
Initial compressive strength [MPa] Compressive strength, after 800⁰C [MPa] 100%N-TMW 7,99 0,00 21,40 100%WG 7,45 16,36 0,00 100%MK 13,67 20,42 17,84 80%N-TMW+10%WG-10%MK 11,08 10,58 29,06 80%N-TMW+20%WG 8,71 3,70 30,48 80%N-TMW+20%MK 8,82 18,44 24,72 60%N-TMW+20%WG+20%MK 9,93 17,90 23,80 55%N-TMW+27%WG+18%MK 10,92 21,04 30,26 50%N-TMW+25%WG+25%MK 8,67 30,90 25,98 50%WG+50%MK 10,03 21,40 34,34 80%N-TMW+10%WG+10%MK+10%GC 8,69 10,44 26,52 80%N-TMW+10%WG+10%MK+20%GC 8,86 7,63 28,98 60%N-TMW+20%WG+20%MK+10%GC 8,59 17,38 23,56 55%N-TMW+27%WG+18%MK+10%GC 10,68 19,80 26,12 55%N-TMW+27%WG+18%MK+20%GC 11,07 10,94 41,54
3.4. Concrete compressive strength and elastic modulus
(TCW) was also determined in this study. Seven prisms and one cube were subjected to the tests at the 28th day. The elastic modulus (EM) results are presented in table 4. It shows a
variation between 1.20 to 7.96 GPa. The EM was obtained by three different Standard calculation methods: The ASTM method with a result of 3.13 GPa, per European Standard with values of 5.28 GPa and 4.75 GPa and per LNEC method a value of 4.30 GPa. The overall average of the results was 4.36 GPa. The presented results show a five times smaller elastic modulus when compared with the elastic modulus or an ordinary Portland cement concrete through the standard ACI 318-89 which is 22.30 GPa . Therefore, results indicate that AAC is more elastic than ordinary Portland cement concrete.
Table 4. Elastic modulus of AAC produced with TCW
ACC specimen Compressive strength (MPa)
Elastic Modulus (GPa)
ASTM E ASTM ASTM
C,0 = EC,S (A) EC,S (B) Prism 1 25.09 3.40 5.35 4.25 3.85 Prism 2 23.90 3.95 4.70 4.23 3.81 Prism 3 21.40 2.82 3.86 3.51 3.23 Prism 4 17.27 3.24 3.87 3.27 3.38 Prism 5 26.52 1.20 7.96 7.07 6.52 Prism 6 19.09 1.65 5.15 5.14 4.60 Prism 7 22.71 5.65 6.07 5.77 4.69 Average 22.28 3.13 5.28 4.75 4.30
4. Innovative applications
4.1 Modular system for vegetated surfaces
GEOGREEN is a modular system of prefabricated elements with vegetation, suitable for new buildings and retrofitting. Its concept is based in a new design for a modular living wall system (LWS) which incorporates industrial waste materials and industrial sub-products. Each module includes a base in an alkali activated material (AAM) and a top layer of expanded cork board (ICB). These modules were designed to be adaptable to different supports, and to obtain a continuous and uniform layer of vegetation. The system can be applied manually and each module can be easily removed for maintenance purposes. The materials and plants used in the system aim to minimize the irrigation needs, to improve buildings thermal behaviour  and their acoustic conditions .
Figure 2. GEOGREEN module: with lower layer in alkali-activated binder (a) and upper layer in expanded cork with circular openings (b).
The alkali activated precast base used in this system is obtained from the mixture of two industrial wastes used as precursors, mine waste mud from Panasqueira mine and milled glass. Milled glass is used to increase the amount of amorphous material in the mixture. The binary blend is activated using a composite activator based on a mixture of sodium silicate and sodium hydroxide. Expanded cork granules are also added to the mixture. They are a lightweight aggregate which result from the crushing of waste expanded cork agglomerate. In the alkali activated mixture they are used to reduce the binder density and increase its water absorption. The mixture is casted into a plastic mold and subject to a curing process in a ventilated oven at 60ºC during 7 days.
Several alkali-activated mixtures were prepared using different variables and aggregates . Variables as percentage substitution of mine waste per glass waste, molar concentration of sodium hydroxide, cure length and temperature, were tested to identify the reference mixture. After these tests, different percentages of aggregates as sand, expanded cork granules and expanded clay were added to reference mixture. Results indicate that the mixture with 25% of sand obtained the maximum compressive strength of 35MPa after 7 curing days. Capillary absorption coefficient can reach to 4,77 kg/m2.h0,5 when adding 25% of cork granules and to
4,11 kg/m2.h0,5 with when adding 25% of sand. Also, if the addition of cork granules is increased
to 50% it enables a 20% density reduction when compared to the reference mixture.
4.2. Alkali-activated foamed materials
Recently, novel ideas have been proposed for the manufacture of alkali-activated foamed materials to produce lightweight materials combining the performance and the benefits of energy saving with the emission reductions obtained [20,26] . The two main ways of producing foamed materials are by introducing mechanically pre-formed foam into the binder or by using a chemical foaming technique.
Fig…. Photographs of alkali-activated foam sample.
Alkali-activated materials have been foamed for suitable thermal conductivity and low density for the application of new types of thermal insulation materials .The processes used to manufacture alkali-activated foam materials have been the same as for conventional aerated concrete, i.e. pre-foaming or mixed foaming [28,29]. Nevertheless, the porosity and thermal insulation properties of alkali-activated foamed materials prepared by the mixed foaming process have not exceeded those of traditional porous materials such as glass foam or autoclaved aerated concrete. Currently, these are the problems limiting the use of
alkali-activated foam as alternative thermal insulation materials to compete with traditional porous inorganic materials.
Besides foaming, density reduction of alkali-activated materials can be done by using lightweight aggregate as alternative to the normal weight granules, where they show better thermal insulating features . Expanded granulated cork has been studied in various industries as lightweight aggregate and the fact that cork is a natural product their usage has eco-efficient advantages [31,32].
This research was partially supported by European Commission under Horizon 2020, Marie Skłodowska-Curie Actions, Research and Innovation Staff Exchange (RISE), by REMINE – “Reuse of Mining Waste into Innovative Geopolymeric-based Structural Panels, Precast, Ready Mixes and Insitu Applications”. Project no 645696 (https://reminemsca.wordpress.com). It was also financed by FCT - Foundation for Science and Technology, IP, within the research unit C-MADE, Centre of Materials and Building Technologies (https://cmadeubi.wordpress.com), University of Beira Interior, Portugal.
 S. Usha, D.G. Nair, S. Vishnudas, Geopolymer Binder From Industrial Wastes: A Review, Int. J. Civ. Eng. &Technology. 5 (2014) 219–225.
 L.K. Turner, F.G. Collins, Carbon dioxide equivalent (CO2-e) emissions: A comparison between geopolymer and OPC cement concrete, Constr. Build. Mater. 43 (2013) 125– 130. doi:10.1016/j.conbuildmat.2013.01.023.
 D.N. Huntzinger, T.D. Eatmon, A life-cycle assessment of Portland cement
manufacturing: comparing the traditional process with alternative technologies, J. Clean. Prod. 17 (2009) 668–675. doi:10.1016/j.jclepro.2008.04.007.
 R.M. Andrew, Global CO2 emissions from cement production, Earth Syst. Sci. Data Discuss. (2017) 1–52. doi:10.5194/essd-2017-77.
 E. Gartner, H. Hirao, A review of alternative approaches to the reduction of CO2 emissions associated with the manufacture of the binder phase in concrete, Cem. Concr. Res. 78 (2015) 126–142. doi:10.1016/j.cemconres.2015.04.012.
 J. Davidovits, Global Warming Impact on the Cement and Aggregates Industries, World Resour. Rev. 6 (1994) 263–278.
 J.L. Provis, J.S.J. van Deventer, Geopolymers - Structure, Processing, Properties and Industrial Applications, Woodhead Publishing Limited, 2009.
 Eurostat, Waste statistics Main statistical findings Total waste generation, 2012 (2016).
 H. Hebhoub, H. Aoun, M. Belachia, H. Houari, E. Ghorbel, Use of waste marble aggregates in concrete, Constr. Build. Mater. 25 (2011) 1167–1171.
 F. Raupp-Pereira, R.J. Ball, J. Rocha, J. Labrincha, G. Allen, New waste based clinkers: Belite and lime formulations, Cem. Concr. Res. 38 (2008) 511–521.
 J.P. Castro-Gomes, A.P. Silva, R.P. Cano, J. Durán Suarez, a. Albuquerque, Potential for reuse of tungsten mining waste-rock in technical-artistic value added products, J. Clean. Prod. 25 (2012) 34–41. doi:10.1016/j.jclepro.2011.11.064.
 F. Pacheco-Torgal, J.P. Castro-Gomes, S. Jalali, Utilization of mining wastes to produce geopolymer binders, in: J.L. Provis, J.S.J. van Deventer (Eds.), Geopolymers - Struct. Process. Prop. Ind. Appl., Woodhead Publishing Limited, 2009: pp. 267–293.  I. Silva, J.P. Castro-Gomes, A. Albuquerque, Effect of immersion in water partially
alkali-activated materials obtained of tungsten mine waste mud, Constr. Build. Mater. 35 (2012) 117–124. doi:10.1016/j.conbuildmat.2012.02.069.
Fernández-Jiménez, Activación alcalina: Revisión y nuevas perspectivas de análisis, Mater. Construcción. 64 (2014) e022. doi:10.3989/mc.2014.00314.
 J.L. Provis, A. Palomo, C. Shi, Advances in understanding alkali-activated materials, Cem. Concr. Res. 78 (2015) 110–125. doi:10.1016/j.cemconres.2015.04.013.
 N. Sedira, J. Castro-Gomes, G. Kastiukas, X. Zhou, A. Vargas, A review on mineral waste for chemical-activated binders: mineralogical and chemical characteristics, Min. Sci. 24 (2017) 29–58. doi:10.5277/MSC172402.
 N. Sedira, J. Castro-Gomes, G. Kastiukas, X. Zhou, A. Vargas, A review on mineral waste for alkali-activated binders due to their chemical characteristics, Min. Sci. 24 (2017) 29–58. doi:10.5277/msc172402.
 REMINE | H2020-MSCA-RISE-2014, (https://reminemsca.wordpress.com).
 C. Sangiorgi, C. Lantieri, P. Tantaranni, J. Castro-Gomes, M. Gabriel, Reuse of mining waste into innovative alkali-activated-based materials for road pavement applications, in: S. Erkens, X. Liu, K. Anupam, T. Yiqiu (Eds.), Funct. Pavement Des. Proc. 4th Chinese-European Work. Funct. Pavement Des. (4th CEW 2016, Delft, Netherlands, 29 June - 1 July 2016)., CRC Press, 2016: p. 204. doi:doi:10.1201/9781315643274-181.  I. Beghoura, J. Castro-Gomes, H. Ihsan, N. Estrada, Feasibility of alkali-activated
mining waste foamed materials incorporating expanded cork, Min. Sci. 24 (2017) 7–28. doi:10.5277/msc172401.
 G. Kastiukas, X. Zhou, J. Castro-Gomes, Preparation conditions for the synthesis of alkali-activated binders using tungsten mining waste, J. Mater. Civ. Eng. 29 (2017). doi:10.1061/(ASCE)MT.1943-5533.0002029.
 A.C.I. ACI, Building code requirements for structural concrete (ACI 318-95), Farmington Hills, 1995.
 M. Manso, J.P. Castro-Gomes, Thermal analysis of a new modular system for green walls, J. Build. Eng. 7 (2016) 53–62. doi:10.1016/j.jobe.2016.03.006.
 M. Manso, J.P. Castro-Gomes, M. Marchacz, M. Górski, L. Dulak, R. Zuchowski,
Acoustic Evaluation of a New Modular System for Green Roofs and Green Walls, Archit. Civ. Eng. Environ. 7 (2017) 99–108.
 M. Manso, J. Castro-Gomes, P. Silva, Modular system design for vegetated surfaces: a proposal for energy-efficient buildings, in: BESS-SB13 Calif. Adv. Towar. Net Zero. Pomona, California, USA., 2013: pp. 1–6.
 Z. Zhang, J.L. Provis, A. Reid, H. Wang, Geopolymer foam concrete: An emerging material for sustainable construction, Constr. Build. Mater. 56 (2014) 113–127. doi:10.1016/j.conbuildmat.2014.01.081.
 J. Henon, A. Alzina, J. Absi, D.S. Smith, S. Rossignol, Potassium geopolymer foams made with silica fume pore forming agent for thermal insulation, J. Porous Mater. 20 (2013) 37–46. doi:10.1007/s10934-012-9572-3.
 P. Hlaváček, V. Šmilauer, F. Škvára, L. Kopecký, R. Šulc, Inorganic foams made from alkali-activated fly ash: Mechanical, chemical and physical properties, J. Eur. Ceram. Soc. 35 (2015) 703–709. doi:10.1016/j.jeurceramsoc.2014.08.024.
 J.A. Bogas, D. Cunha, Non-structural lightweight concrete with volcanic scoria
aggregates for lightweight fill in building’s floors, Constr. Build. Mater. 135 (2017) 151– 163. doi:10.1016/j.conbuildmat.2016.12.213.
 A. Brás, M. Leal, P. Faria, Cement-cork mortars for thermal bridges correction. Comparison with cement-EPS mortars performance, Constr. Build. Mater. 49 (2013) 315–327. doi:10.1016/j.conbuildmat.2013.08.006.
 S.R. Karade, M. Irle, K. Maher, Influence of granule properties and concentration on cork-cement compatibility, Holz Als Roh - Und Werkst. 64 (2006) 281–286.
 P.J.R.O. Nóvoa, M.C.S. Ribeiro, A.J.M. Ferreira, A.T. Marques, Mechanical characterization of lightweight polymer mortar modified with cork granulates, Compos. Sci. Technol. 64 (2004) 2197–2205. doi:10.1016/j.compscitech.2004.03.006.